Please cite this article as follows:Ghadirian H, Geramy A, Shallal W, Heidari S, Noshiri N, Keshvad MA. The effect of remineralizing doi 10.34172/jlms.2020.25
The Effect of Remineralizing Agents With/Without
Laser Irradiation on Structural and Mechanical
Properties of Enamel and its Shear Bond Strength to
Hannaneh Ghadirian1, Allahyar Geramy1, Waleed Shallal2, Soolmaz Heidari3, Nooshin Noshiri4, Mohammad Ali Keshvad1*
1Department of Orthodontics, School of Dentistry, Tehran University of Medical sciences, Tehran, Iran 2Al Karama Teaching Hospital, Kut, Iraq
3Department of Operative Dentistry, Dental Caries Prevention Research Center, Qazvin University of Medical Sciences,
4Medical Image Processing Laboratory (MIPL), Department of Technology and Engineering, Alzahra University, Tehran, Iran
Introduction: Remineralizing agents may be used for the treatment of white spot lesions (WSLs) prior to bracket bonding. However, some concerns exist regarding their possible interference with the etching and bonding process, negatively affecting the bond strength. This study aimed to assess the effect of two remineralizing agents with/without CO2 laser irradiation on the mechanical properties and shear bond strength (SBS) of demineralized enamel to the orthodontic bracket.
Methods: This study evaluated 60 premolar teeth in 6 groups (n=10) as follows: (I) sound enamel, (II) demineralized enamel, (III) Nupro remineralizing agent (N), (IV) Nupro and CO2 laser (N/L), (V) Teethmate remineralizing agent (T), and (VI) Teethmate and CO2 laser (T/L). The remineralizing agents were applied to the enamel surfaces after their immersion in a demineralizing solution for 5 days. In groups IV and VI, the CO2 laser with a 10.6 μm wavelength, 10 ms pulse duration, a 50 Hz repetition rate, 0.3 mm beam diameter and 0.7 W power was irradiated after applying the remineralizing agents. Brackets were bonded to the enamel surfaces and SBS was measured by a universal testing machine. For the assessment of enamel microhardness, 20 sections of molar teeth were divided into 4 groups (n=5; N, N/L, T, T/L) and their microhardness was measured before demineralization, after demineralization and after remineralization. X-ray diffraction (XRD) analysis, field-emission scanning electron microscopy (FESEM) and energy-dispersive spectrometry (EDS) were carried out to assess the formation of hydroxyapatite. The atomic percentages of the C, O, P, Ca, Na, Si, F and Ca/P ratio were determined by EDS analysis.
Results: The SBS significantly decreased in group II (P < 0.001). There was no significant difference among the groups I, III, IV, V and VI (P < 0.05). This finding was similar to the microhardness results, which showed an increase in microhardness after remineralization (P < 0.05), with no difference among the remineralizing agents. The Ca/P ratio was the highest in the Nupro group and the lowest in the demineralized group.
Conclusion: Remineralizing agents can significantly improve the microhardness and structural properties of demineralized enamel to a level similar to that of sound enamel with no adverse effect on SBS to orthodontic brackets.
Keywords: White spot; CO2 Laser; Shear strength; Nupro; Teethmate; X-ray diffractions.
Mohammad Ali Keshvad, Department of Orthodontics, School of dentistry, North Kargar St, Tehran, Iran.
Tel: +989128026404; Email:
Published online March 15,
in Medical Scienceshttp://journals.sbmu.ac.ir/jlms
Orthodontic treatment is performed aiming to improve function, esthetics, and stability. Despite the favorable functional and esthetic results of orthodontic treatment with fixed appliances, this treatment may have unfavorable consequences such as periodontal disease and dental caries, particularly in patients with poor oral hygiene. Furthermore, the presence of archwires, brackets and
bands can complicate oral hygiene practice in orthodontic patients.1 Organic acids caused by acidogenic bacteria can dissolve the enamel minerals and cause porosities in the tooth surface, leading to initial carious lesions known as the white spot lesions (WSLs).2
Most studies have reported a prevalence of 23%-73% for WSLs in orthodontic patients, depending on treatment duration.3-5 Several strategies such as patient education to
maintain good oral hygiene,6 the application of adhesives
containing remineralizing agents,7 and the prophylactic
use of fluoride varnishes8 have been suggested to
minimize the development of WSLs. In addition to these preventive methods, the use of remineralizing agents is recommended before and during orthodontic treatment, especially for patients who have demineralized enamel prior to the onset of treatment. Some studies have reported a reduction in bond strength when fluoride or casein phosphopeptide amorphous calcium phosphates (CPP-ACP) were applied as a remineralizing agent before acid-etching, while some others did not confirm the adverse effects of remineralizing agents on bond strength of brackets.9-13
CPP-ACP can be used intraorally to deliver high concentrations of bioavailable calcium and phosphate ions, prevent demineralization and enhance remineralization as such. The cariostatic activity of CPP-ACP is related to the ability of CPP to localize ACP on the tooth surface and increase the calcium and phosphate levels in dental plaque.14
Bioactive glass has been introduced for dental prophylaxis, and many studies have attempted to remineralize the demineralized enamel using bioactive
glass.15-17 Bioactive glass reacts with saliva to release
Ca2+, Na+, and PO
43− ions.18 It forms a layer highly reach in calcium, phosphate and silica attached to the enamel surface and thus has the potential to remineralize the tooth structure.19
Many laser types are also used for preventive purposes in dentistry. The CO2 laser is suitable for use on enamel surfaces because its wavelength is within the infrared spectrum and is absorbed by phosphate and carbonate
bands.20 The CO
2 laser plays an important role in
caries prevention with insignificant adverse effects
on tooth structure.21 Laser irradiation generates heat,
which modifies the carbonated hydroxyapatite by the fusion of hydroxyapatite crystals, and the reduction of interprismatic spaces in the enamel structure.22,23
Decreased shear bond strength (SBS) can lead to bracket debonding, cause problems for both the clinician and patient, increase the treatment cost, and prolong the course of treatment. Therefore, it is essential to find out whether the remineralizing agents have the ability to treat the demineralized enamel with no adverse effect on their SBS to orthodontic brackets. A safe material should not decrease the bond strength lower than 6 to 8 MPa, which is the minimum bond strength required for orthodontic bracket bonding.24,25
This study aimed to evaluate the effect of two
remineralizing agents with and without CO2 laser
irradiation on the structural characteristics of demineralized enamel and its SBS to orthodontic brackets. Materials and Methods
Sixty Extracted human premolars were used for the
evaluation of SBS while 10 extracted molars were used for the evaluation of microhardness following demineralization and remineralization processes. The enamel disc-shaped samples were also used to evaluate the structural changes. The exclusion criteria were the presence of caries, cracks, erosion, fluorosis, hypo-calcification and dental restorations. The teeth had normal buccal and lingual surface morphology and were extracted atraumatically. All the teeth were cleaned from debris and soft tissue remnants and they were polished with non-fluoride pumice paste and rubber cups with a low-speed hand-piece. Then they were stored in a 0.5% chloramine-T solution for 7 days for disinfection.26
Ten molar teeth were decoronated at the cementoenamel junction, and each crown was longitudinally sectioned in half in the occlusogingival direction using a water-cooled, high-speed saw (Mecatome T201; Presi, France) to obtain buccal and lingual enamel samples with 2-3 mm thickness. Twenty enamel samples obtained as such were mounted in a custom-made wax mold and polished with 800, 1200, 1600 and 2000-grit silicon carbide discs under water coolant to obtain flat enamel surfaces. Two layers of nail varnish were applied to cover the enamel surface, leaving a window of about 4×4 mm for demineralization and remineralization processes.
Demineralization and Remineralization Processes
Twenty enamel samples were divided into 4 groups and underwent demineralization and remineralization processes. The microhardness of the surface was measured in each step using a microhardness tester (Vickers pyramid diamond indenter, MH Tester device, Bareiss, Germany) by applying a 100 g load for 8 seconds. In order to decide upon the proper time for the demineralization process, a pilot study was carried out. According to the obtained results, 5 days of immersion in demineralizing solution was chosen as the proper time to demineralize the enamel surface (a decrease in microhardness value by less than 50%). To evaluate the remineralization ability, the samples were treated with the respective remineralizing agents according to the manufacturers’ instructions. The protocols of the application of remineralizing agents were as follows:
• Nupro (N) and Nupro/laser (N/L) groups: Nupro prophy paste was applied to demineralized enamel surfaces using a micro-brush with a rotational movement for 1 minute. The approximate thickness of the paste was nearly 2 mm.
• Teethmate (T) and Teethmate/laser (T/L) groups: The powder and liquid of the Teethmate remineralizing agent were mixed for 15 seconds. The slurry paste was applied to enamel surfaces by a brush in 2 mm thickness for 30 seconds and it was left to dry.
In laser groups, after applying the remineralizing
agents, the pulsed CO2 laser (Smart US-20D, Deka, Italy)
was irradiated with a 10.6 μm wavelength, 10 ms pulse duration, a 50 Hz repetition rate, 0.3 mm beam diameter and 0.7 W power in a scanning motion for 10 seconds with a 5 mm distance away from the enamel surface.
Before immersion in remineralizing solution, a thin layer of a 7th generation bonding agent (Clearfil Tri-S Bond, Kuraray, Noritake Dental Inc., Okayama, Japan) was applied passively over the remineralizing agents to
protect them from being washed-out.27,28 The adhesive
was applied for 20 seconds and cured using a light-curing unit for 10 seconds. The samples of each group were individually stored in glass containers containing artificial saliva as a remineralizing agent for 7 days.
At the end of the storage period, the adhesive layer that covers the remineralizing agents was gently removed with a tweezer. The samples were then rinsed with deionized water. The surface microhardness of all samples was measured after the remineralization process, similar to the aforementioned protocol. The composition of materials and solutions used for demineralization and remineralization processes is presented in Table 1.
In order to evaluate hydroxyapatite formation, X-ray diffraction analysis (XRD), field-emission scanning electron microscopy (FESEM), and energy-dispersive spectrometry (EDS) were carried out. The enamel
samples of molar teeth were prepared according to the method described for the microhardness test.
The XRD (X’Pert PRO-MPD, PANalytical Company, Netherlands) analysis was performed using Cu Kα radiation (k = 1.542 Å) operating at 40 mA and 40 kV in the range of 10-110° 2θ with continuous scanning. FESEM (MIRA3 TESCAN-XMU, Czech Republic) coupled with EDS (SAMX, France) with an accelerated voltage of 15 kV was carried out to assess the morphological changes of the enamel surface and identify elemental changes in the enamel surface of each sample. For FESEM, the enamel samples were cleaned with acetone, dehydrated with ethanol (at a gradient concentration of 70%, 80%, 90%, and 100% for 20 minutes) and left to dry at room temperature for 24 hours. The samples were then sputter-coated with gold.
Shear Bond Strength
Sixty premolars were randomly divided into 6 groups (sound enamel, demineralized enamel, N, N/L, T, and T/L). The remineralizing agents were applied as explained earlier. After the demineralization and remineralization processes, orthodontic brackets were bonded to premolars. Premolar stainless steel brackets (Discovery®, Dentaurum, Ispringen, Germany) were positioned at the center of the buccal surface of the anatomic crown and bonded
using Transbond™ XT light-cure adhesive (3M Unitek,
Monrovia, CA, USA) according to the manufacturer’s instructions. Before photo-polymerization, each bracket
Table 1. Composition of Materials and Solutions Used for Demineralization and Remineralization Processes
Material Company Composition Lot. No. Method of Application
solution Hand mixing CaCl2, NaCl, NaH2PO4, NaN3, Acetic acid Immersion with 5 days
solution Hand mixing CaCl2, NaCl, NaH2PO4, NaN3 Immersion with 7 days
Nupro prophy paste
Dentsply professional (UAS)
45S5 Bioactive glass (wt%):
45%SiO2,24.5%Na2O, 24.5%CaO, 6%P2O5
801227 Apply with rotational mixing for 1 min and cover with a bond for 7 days
Teethmate Kuraray Noritake Dental Inc. (Japan)
Tetra-calcium phosphate, Di-calcium phosphate anhydrous
2) Liquid: Water, Preservative
Mix the powder and liquid for 15 s and apply for 30 s and then cover with a bond for 7 days
Clearfil Tri-S Bond Kuraray Noritake Dental Inc. (Japan)
Bis-GMA, MDP, HEMA, hydrophilic aliphatic dimethacrylate, hydrophobic aliphatic methacrylate, colloidal silica, CQ, ethanol, water
Apply passively over the remineralizing materials for 20 s and then light-cured for 10 s.
Primer 3M Unitek (Germany)
4-dimethylaminobenzene, ethanol, CQ, hydroquinone
REF 712-035 Apply a thin layer to enamel Transbond XT
Composite 3M Unitek (Germany)
Bis-GMA, Bis-EMA, Acrylate, Monomers,
Filler REF 712-035
Apply to the bracket base, positioning of the bracket and then light-cured for 40 s. Unitek Etching Gel 3M Unitek (Germany) 35% Phosphoric acid REF 704-060 Apply for 15 s on the enamel and wash
for 15 s with water-air spray
Nail Varnish Iran Acid-resistant paint Apply over surfaces and leave to dry
Abbreviations: Bis-GMA: bisphenol A diglycidylmethacrylate; MDP: 10-methacryloyloxydecyl dihydrogen phosphate; HEMA: 2-hydroxyethyl methacrylate; NaF: sodium fluoride; CQ: campherquinone; TEG-DMA: triethyleneglycol dimethacrylate; Bis-EMA: ethoxylated bis-phenol-A-glycol dimethacrylate.
was subjected to 300 g compressive force by using a force gauge (Correx Co, Berne, Switzerland), as previously
described by Bishara et al.29 The excess adhesive paste
was removed with a small scaler from the margins of the bracket base. All brackets were light-cured for 40 seconds
with a dental light-curing unit with 1200 mW/cm2
intensity. Thermocycling (thermo-cycling device, TC 300, Vafaei Industrial, Iran) was performed for 1500 cycles in deionized water between 5-55°C with 30 seconds of dwell time30,31 to simulate the oral environment. The roots were embedded in a cubic mold of auto-polymerizing acrylic resin (Acro-pars, Iran) using a mounting jig and a 0.019×0.025 inch straight stainless steel wire to align the buccal surface of each tooth perpendicular to the base of the mold. For SBS testing, the samples were secured in the lower jaw of a universal testing machine (Zwick/ Roell Z050, Ulm, Germany) such that the bracket base of the sample paralleled the direction of the shear force. The samples were stressed in an occlusogingival direction with
a cross-head speed of 1 mm/min.13,32 After debonding,
the teeth were inspected under a stereomicroscope (SMZ 800, Nikon, Japan) at ×10 magnification to quantify the remaining adhesive, according to the modified adhesive
remnant index (ARI).33 The ARI scores ranged from 1 to
5 as described in Table 2.
For surface microhardness evaluation, repeated measures ANOVA followed by a Bonferroni t-test were carried out for pairwise comparisons. A one-way ANOVA and a post-hoc Tukey’s test were performed to analyze the SBS data. The differences in ARI scores were analyzed by the
Kruskal-Wallis test. P < 0.05 was considered significant. All tests and statistical analyses were carried out using SPSS version 20.
According to Table 3, the results revealed that the demineralization process caused a significant reduction in the mean microhardness. There was a significant increase in the mean microhardness after the application of remineralizing agents in all groups (P < 0.05). The ability to improve the condition from demineralization to remineralization was not significant in different groups and the results showed no statistically significant difference among the remineralization groups. However, microhardness values were higher in laser groups (N/L and T/L) compared to no laser groups (N and T).
Figure 1 shows the characteristic peaks of the XRD pattern. The peaks (002) at 2θ = 26 and (211) at 2θ = 32.2 are specific peaks for hydroxyapatite in the XRD pattern according to the reference database of the XRD pattern.34,35 The sound enamel group showed typical characteristics of hydroxyapatite crystals. To compare the spectra of the groups, the ratio of the diffraction peak intensities (002/211) was calculated. This ratio was 2.79 for the sound enamel while it was 3.48 for the demineralized enamel. The obtained ratios for the remineralized enamel in N, N/L, T and T/L groups were 2.78, 2.82, 2.74, and 3.01 respectively.
Table 2. The Ranges of Adhesive Remnant Index (ARI) Scores Score Criteria
1 All the adhesive, with tooth impression of the bracket base, remained on the tooth 2 More than 90% of the adhesive remained on the tooth
3 More than 10% but less than 90% of the adhesive remained on the tooth 4 Less than 10% of the adhesive remained on the tooth
5 No adhesive remained on the tooth
Table 3. Means and Standard Deviation of Vicker’s Microhardness Number for Different Remineralizing Agents
Groups N Stages Minimum Maximum Mean Standard Deviation
5 Sound enamel 315 457 393.00 54.424
5 Demineralized enamel 64 100 81.00 16.763
5 Remineralized enamel 134 225 185.00 33.756
Nupro and laser
5 Sound enamel 395 473 441.80 31.060 5 Demineralized enamel 87 127 107.60 14.792 5 Remineralized enamel 187 247 219.00 22.327 Teethmate 5 Sound enamel 260 413 362.60 63.752 5 Demineralized enamel 49 104 82.40 22.534 5 Remineralized enamel 114 225 166.00 49.209
Teethmate and laser
5 Sound enamel 313 482 402.60 60.682
5 Demineralized enamel 85 110 101.80 10.803
The XRD pattern and the peak intensity ratio of the remineralized enamel in all the groups were closer to the sound enamel than the demineralized enamel.
Figure 2 shows the FESEM patterns of the groups. For the sound enamel, a homogeneous smooth appearance with no irregularity was seen. The demineralized enamel surface was rough and eroded. In group N, porosities were covered with a hydroxyapatite deposit. However, the underlying pattern was still visible in some areas. In group N/L, the underlying pattern could not be seen, while a melted and welded appearance caused by laser irradiation was observed. In group T, the enamel surface was entirely covered with granular-shaped hydroxyapatite deposits, while in group T/L, the enamel surface was covered with relatively smooth and more homogeneous crystalline structure compared to group T, due to the typical melting effect of the laser. Figure 2 also shows the chemical composition and atomic percentages of C, O, P, Ca, Na, Si, and F in the groups. The hydroxyapatite deposit was confirmed by EDS analysis in all the groups. The effect of demineralization and remineralization protocols on the enamel surface composition was evaluated by measuring the Ca/P ratio, which was the highest for the Nupro group and the lowest for the demineralized group.
Shear Bond Strength
As indicated in Table 4, the results showed that the SBS was significantly lower in the demineralized group compared to all other groups (P < 0.001), while there was no significant difference among other groups (P > 0.05). The laser groups showed SBS values lower than the groups without the laser. Table 5 lists the ARI scores for the 6 groups. The demineralized groups showed ARI score 5 in 4 samples out of 10, which was in agreement with the results of the SBS test.
Teethmate and Nupro prophy paste were the remineralizing
Figure 1. The XRD Pattern of Sound Enamel, Dem (Demineralized), N
(Nupro), N/L (Nupro and Laser), T (Teethmate), T/L (Teehtmate and Laser).
Figure 2. FESEM Images and EDS Analysis of Sound Enamel (a),
Demineralized Enamel (b), Nupro (c), Nupro and Laser (d), Teethmate (e), Teethmate and Laser (f).
agents evaluated in this study. Teethmate is composed of two different types of calcium phosphate (tetracalcium phosphate and dicalcium phosphate anhydrous) which
react with water to form hydroxyapatite.36,37 Nupro
bioactive glass is mainly composed of SiO2, Na2O, CaO, and P2O5. According to a study by Gupta et al, sodium release can increase the local pH and facilitate the deposition of
additional phosphate and calcium ions.27,38 Due to the
possible role of the CO2 laser in the remineralization
process, the CO2 laser has also been used to evaluate the probable synergistic effect of the laser on remineralizing agents.22,39 The safety of controlled irradiation of the CO
2 laser for the pulp and dental structures has previously been confirmed.40,41
The chemical analyses of enamel surfaces by EDS revealed that the dominant elements were oxygen (O), carbon (C), calcium (Ca), and phosphorus (P). These elements are the main components of enamel structure and comprise the standard composition of hydroxyapatite. The Ca/P ratio of the sound enamel (1.56 %) decreased to 1.32 % for the demineralized enamel. This obvious difference may refer to the amount of calcium and phosphorus leached out from the enamel during the demineralization
process. This finding was consistent with FESEM images that showed porosities on the enamel surface following the demineralization process. The Ca/P ratios were elevated in all the study groups after the treatment with remineralizing agents and were nearly similar to that of intact enamel with the highest percentage in the N group (1.62%). It means that the nature and pattern of the formed crystals were more similar to those of the intact enamel compared to the demineralized enamel, which was also confirmed by XRD results. This finding was approved by FESEM images, which showed the formation of the HA deposit on the demineralized enamel.
The comparison between the laser-irradiated and non-irradiated groups showed no significant effect of the laser on atomic percentages of Ca and P. The atomic Ca/P ratios for the laser groups showed that laser irradiation had no additional effect on the uptake of calcium and phosphate when combined with the remineralizing agents. On the other hand, El Assal et al indicated that the combination of the CO2 laser with the hydroxyapatite nano-particles as a remineralizing agent increased the percentage of Ca and P.42 This synergetic effect is ascribed to the heat produced
by the CO2 laser which can melt the enamel surface and
link the remineralizing agent to the enamel surface. The
higher power density applied (more than 3 W/cm2) may
be an explanation for this controversy.43 Clearly visible on FESEM images, the laser facilitated the fusion of the formed hydroxyapatite deposit with the enamel.
According to the findings of FESEM, the sound enamel showed a homogeneous and smooth appearance due to the unexposed enamel rods. In the demineralized enamel, the rough surface was attributed to the exposed
Table 4. Means and Standard Deviation of Shear Bond Strength (MPa) for the Study Groups
Groups No Samples Minimum Maximum Mean Standard Deviation
Sound enamel 10 23.56 38.21 28.9820 5.23600
Demineralized enamel 10 9.17 22.35 16.9760 5.07002
Nupro 10 15.17 43.27 30.9750 7.92504
Nupro and laser 10 19.69 29.23 25.0990 3.30448
Teethmate 10 15.41 38.98 29.0990 6.23642
Teethmate and laser 10 19.62 35.85 27.7820 6.14152
Table 5. Adhesive Remnant Index (ARI) Scores of the Study Groups
1 2 3 4 5
Sound enamel 0 2 3 5 0
Demineralized enamel 0 0 1 5 4
Nupro 0 1 6 3 0
Nupro and laser 0 1 4 5 0
Teethmate 0 0 7 3 0
Teethmate and laser 0 2 4 4 0
Total 0 6 25 25 4
hydroxyapatite rods following the removal of peripheral enamel prisms. The more homogeneous enamel surface in the laser groups was related to the coalescence of enamel prisms with each other and with mineral deposits. This finding can be related to the EDS results showing Ca/P ratios similar to those found in the sound enamel. Similar to the study by Ahrari et al, the groups treated with the remineralizing agents alone showed non-homogenous layers with granular or globular precipitations covering
the underlying enamel surface.44
In XRD analysis, the intensity of diffraction peaks was calculated to compare the hydroxyapatite pattern of the sound enamel, enamel after demineralization, and enamel after remineralization in all groups. The demineralized samples showed an increased intensity of 002 peak, indicative of the improved rearrangement of hydroxyapatite crystals along the c-axis due to the greater removal of hydroxyapatite crystals from the peripheral
enamel prisms compared to the core area.45 The XRD
pattern of the treated samples showed a similar pattern to the natural enamel. The comparison of the laser groups and the sound enamel showed that the laser had no significant effect on enamel structure. This finding was in agreement with the results of Nakagaki et al,
who showed no change in enamel structure by CO2 laser
irradiation (0.5 W output power for 1 minute) following the use of fluoride. However, laser irradiation with 4 W output power for 1 minute resulted in the formation of
an amorphous-like structure.46 Furthermore, Lin et al
showed that the exposure of enamel surface to the CO2
laser (5 W output power for 5 seconds) did not affect the XRD pattern except for the formation of a small
peak of α-TCP.43 It seems that the phase changes of the
enamel surface following exposure to the CO2 laser highly depended on laser parameters.
The mean surface microhardness values showed that there was a significant decrease in the microhardness of the enamel surface after demineralization. This result was in accordance with the elements leached out from the enamel, determined by EDS. Previous studies have also reported a reduction in the hardness of demineralized
enamel.47-49 The significant increase in microhardness
after the remineralization procedure indicates a direct correlation between the Ca/P ratio and the subsequent
surface microhardness of remineralized enamel. According to Amaechi et al, the remineralization of eroded enamel by saliva can take 28 days but as shown by our results, applying remineralizing agents can significantly accelerate this process.50 It has been demonstrated that the materials with high amounts of calcium and phosphate have high penetration into enamel lesions and as a result, greater remineralization occurs. The ability of bioactive glass to penetrate deeper into the demineralized enamel and improve remineralization in comparison with fluoride was approved by the microhardness test by Bakry et al.19 Due to the porous and fragile structure of initial carious lesions, only some studies support the use of lasers alone and without the use of remineralizing agents. Furthermore, it was proposed that the heat generated during laser irradiation can effectively fuse the
loosely-attached layer formed on the enamel surface.51 Despite
the higher microhardness values obtained in the laser groups, the differences were not significant. As a result, the synergistic effect of the laser with the remineralizing agents was not evident in our findings, which is similar to the findings from the study by Farhadian et al.52 Melting and recrystallization of the enamel surface may explain higher microhardness values and also the higher intensity of HA peaks for the laser groups. Contrary to our findings, Khamverdi et al and Niyazi et al showed a synergistic
effect of the CO2 laser with CPP-ACP on improving the
enamel microhardness, which confirms the facilitating role of lasers in the penetration of remineralizing agents into deeper layers of HA.39,53
Calcium-phosphate derivatives transform the hydroxyapatite to stronger crystals by incorporating fluoride into subsurface enamel, which can increase the hardness of demineralized enamel and impede the
demineralization process.54 As a result, both Nupro and
Teethmate can increase the resistance of demineralized enamel to further demineralization while the laser can cause welding of enamel prisms; therefore, the application of these materials combined with laser irradiation can interfere with the etching process and decrease the bond strength. The remineralization mechanism may interfere with the acid-etching process, prevent the production of enamel tags, and decrease the bond strength of orthodontic brackets, which means a higher possibility of bracket debonding during the treatment period. Concerning the bond strength, we found that the SBS significantly decreased when the brackets were bonded to the previously demineralized enamel. This result can be explained by the reduction in the mineral content of the demineralized enamel and is supported by the surface microhardness and EDS results. Also, there was a statistically significant improvement in the SBS of the treated groups compared to the demineralized group, similar to the findings from the study by Velİ et al.55 The higher surface microhardness values in the laser groups can also be related to their lower bond strength, although
it was not significant. Different laser settings, the type of remineralizing agent and its frequency and duration of application can explain different results in the literature. The lower bond strength values of the demineralized samples were in agreement with the ARI scores; 40% of the demineralized samples represented score 5, meaning no adhesive remaining on the tooth surface.
According to the results, the application of the remineralizing agents did not interfere with the SBS of orthodontic brackets to enamel and even enhanced the SBS of treated demineralized enamel and improved its structural properties as well. The results of enamel structural analysis, hydroxyapatite formation, and the SBS test were in agreement with each other. The findings indicated that the enamel surface structure has a definite impact on the clinical performance of fixed appliances and the quality of treatment. Future in vivo studies on other commonly used remineralizing agents are required to enhance the existing knowledge about the remineralizing agents and their clinical effects on the performance of orthodontic appliances.
This in vitro study was approved by the ethics committee of Tehran University of Medical Sciences (Ethic code: IR.TUMS.DENTISTRY.REC.1396.2721).
Conflict of Interests
We have no conflict of interest to disclose in the article. References
1. Tanna N, Kao E, Gladwin M, Ngan PW. Effects of sealant and self-etching primer on enamel decalcification. Part I: an in-vitro study. Am J Orthod Dentofacial Orthop. 2009;135(2):199-205. doi: 10.1016/j.ajodo.2008.09.003. 2. Fernández-Ferrer L, Vicente-Ruíz M, García-Sanz V,
Montiel-Company JM, Paredes-Gallardo V, Almerich-Silla JM, et al. Enamel remineralization therapies for treating postorthodontic white-spot lesions: A systematic review.
J Am Dent Assoc. 2018;149(9):778-786.e2. doi: 10.1016/j.
3. Chapman JA, Roberts WE, Eckert GJ, Kula KS, González-Cabezas C. Risk factors for incidence and severity of white spot lesions during treatment with fixed orthodontic appliances. Am J Orthod Dentofacial Orthop. 2010;138(2):188-94. doi: 10.1016/j.ajodo.2008.10.019. 4. Julien KC, Buschang PH, Campbell PM. Prevalence of
white spot lesion formation during orthodontic treatment.
Angle Orthod. 2013;83(4):641-7. doi:
5. Brown MD, Campbell PM, Schneiderman ED, Buschang PH. A practice-based evaluation of the prevalence and predisposing etiology of white spot lesions. Angle Orthod. 2016;86(2):181-6. doi: 10.2319/041515-249.1.
6. Bergstrand F, Twetman S. A review on prevention and treatment of post-orthodontic white spot lesions -
evidence-based methods and emerging technologies. Open
Dent J. 2011;5:158-62. doi: 10.2174/1874210601105010158.
7. Pascotto RC, Navarro MF, Capelozza Filho L, Cury JA. In vivo effect of a resin-modified glass ionomer cement on enamel demineralization around orthodontic brackets.
Am J Orthod Dentofacial Orthop. 2004;125(1):36-41. doi:
8. Gontijo L, Cruz Rde A, Brandão PR. Dental enamel around fixed orthodontic appliances after fluoride varnish application. Braz Dent J. 2007;18(1):49-53. doi: 10.1590/ s0103-64402007000100011.
9. Kim MJ, Lim BS, Chang WG, Lee YK, Rhee SH, Yang HC. Phosphoric acid incorporated with acidulated phosphate fluoride gel etchant effects on bracket bonding. Angle Orthod. 2005;75(4):678-84. doi: 10.1043/0003-3219(2005)75[678:PAIWAP]2.0.CO;2.
10. Meng CL, Li CH, Wang WN. Bond strength with APF applied after acid etching. Am J Orthod Dentofacial Orthop. 1998;114(5):510-3. doi: 10.1016/s0889-5406(98)70170-2. 11. Park SY, Cha JY, Kim KN, Hwang CJ. The effect of casein
phosphopeptide amorphous calcium phosphate on the in vitro shear bond strength of orthodontic brackets. Korean
J Orthod. 2013;43(1):23-8. doi: 10.4041/kjod.2013.43.1.23.
12. Çehreli SB, Şar Ç, Polat-Özsoy Ö, Ünver B, Özsoy S. Effects of a fluoride-containing casein phosphopeptide-amorphous calcium phosphate complex on the shear bond strength of orthodontic brackets. Eur J Orthod. 2012;34(2):193-7. doi: 10.1093/ejo/cjq183.
13. Keçik D, Cehreli SB, Sar C, Unver B. Effect of acidulated phosphate fluoride and casein phosphopeptide-amorphous calcium phosphate application on shear bond strength of orthodontic brackets. Angle Orthod. 2008;78(1):129-33. doi: 10.2319/122506-529.1.
14. Reynolds EC. Casein phosphopeptide-amorphous calcium phosphate: the scientific evidence. Adv Dent Res. 2009;21(1):25-9. doi: 10.1177/0895937409335619. 15. Mehta AB, Kumari V, Jose R, Izadikhah V. Remineralization
potential of bioactive glass and casein phosphopeptide-amorphous calcium phosphate on initial carious lesion: An in-vitro pH-cycling study. J Conserv Dent. 2014;17(1):3-7. doi: 10.4103/0972-0707.124085.
16. Milly H, Festy F, Watson TF, Thompson I, Banerjee A. Enamel white spot lesions can remineralise using bio-active glass and polyacrylic acid-modified bio-bio-active glass powders. J Dent. 2014;42(2):158-66. doi: 10.1016/j. jdent.2013.11.012.
17. Bakry AS, Takahashi H, Otsuki M, Tagami J. Evaluation of new treatment for incipient enamel demineralization using 45S5 bioglass. Dent Mater. 2014;30(3):314-20. doi: 10.1016/j.dental.2013.12.002.
18. El-Wassefy NA. Remineralizing effect of cold plasma and/or bioglass on demineralized enamel. Dent Mater J. 2017;36(2):157-67. doi: 10.4012/dmj.2016-219.
19. Bakry AS, Marghalani HY, Amin OA, Tagami J. The effect of a bioglass paste on enamel exposed to erosive challenge. J Dent. 2014;42(11):1458-63. doi: 10.1016/j. jdent.2014.05.014.
20. Featherstone JD, Barrett-Vespone NA, Fried D, Kantorowitz Z, Seka W. CO2 laser inhibitor of artificial caries-like lesion progression in dental enamel. J Dent Res. 1998;77(6):1397-403. doi: 10.1177/00220345980770060401.
21. Sabaeian M, Shahzadeh M. Simulation of temperature and thermally induced stress of human tooth under CO2 pulsed laser beams using finite element method. Lasers Med Sci. 2015;30(2):645-51. doi: 10.1007/s10103-013-1390-6. 22. Klein AL, Rodrigues LK, Eduardo CP, Nobre dos
Santos M, Cury JA. Caries inhibition around composite restorations by pulsed carbon dioxide laser application.
Eur J Oral Sci. 2005;113(3):239-44. doi:
23. Miresmaeili A, Farhadian N, Rezaei-soufi L, Saharkhizan M, Veisi M. Effect of carbon dioxide laser irradiation on enamel surface microhardness around orthodontic brackets. Am J Orthod Dentofacial Orthop. 2014;146(2):161-5. doi: 10.1016/j.ajodo.2014.04.023.
24. Whitlock BO 3rd, Eick JD, Ackerman RJ Jr, Glaros AG, Chappell RP. Shear strength of ceramic brackets bonded to porcelain. Am J Orthod Dentofacial Orthop. 1994;106(4):358-64. doi: 10.1016/S0889-5406(94)70056-7. 25. Reynolds IR. A review of direct orthodontic
bonding. Br J Orthod. 1975;2(3):171-8. doi: 10.1080/0301228X.1975.11743666.
26. Eliades T, Brantley W. The inappropriateness of conventional orthodontic bond strength assessment protocols. Eur J Orthod. 2000;22(1):13-23. doi: 10.1093/ ejo/22.1.13.
27. Mohanty P, Padmanabhan S, Chitharanjan AB. An in vitro evaluation of remineralization potential of Novamin® on artificial enamel sub-surface lesions around orthodontic brackets using energy dispersive x-ray analysis (EDX).
J Clin Diagn Res. 2014;8(11):ZC88-91. doi: 10.7860/
28. Pinto de Souza SCT, Araújo KC, Barbosa JR, Cancio V, Rocha AA, Tostes MA. Effect of dentifrice containing fTCP, CPP-ACP and fluoride in the prevention of enamel demineralization. Acta Odontol Scand. 2018;76(3):188-94. doi: 10.1080/00016357.2017.1401658.
29. Bishara SE, Gordan VV, VonWald L, Olson ME. Effect of an acidic primer on shear bond strength of orthodontic brackets. Am J Orthod Dentofacial Orthop. 1998;114(3):243-7. doi: 10.1016/s0889-5406(98)70205-1998;114(3):243-7.
30. Haller B, Hofmann N, Klaiber B, Bloching U. Effect of storage media on microleakage of five dentin bonding agents. Dent Mater. 1993;9(3):191-7. doi: 10.1016/0109-5641(93)90119-b.
31. Gale MS, Darvell BW. Thermal cycling procedures for laboratory testing of dental restorations. J Dent. 1999;27(2):89-99. doi: 10.1016/s0300-5712(98)00037-2. 32. Al-Kawari HM, Al-Jobair AM. Effect of different preventive
agents on bracket shear bond strength: in vitro study. BMC
Oral Health. 2014;14(1):28. doi: 10.1186/1472-6831-14-28.
33. Xiaojun D, Jing L, Xuehua G, Hong R, Youcheng Y, Zhangyu G, et al. Effects of CPP-ACP paste on the shear bond strength of orthodontic brackets. Angle Orthod. 2009;79(5):945-50. doi: 10.2319/101108-573.1.
34. Brundavanam RK, Poinern GEJ, Fawcett D. Modelling the crystal structure of a 30 nm sized particle based hydroxyapatite powder synthesised under the influence of ultrasound irradiation from X-ray powder diffraction data. Am J Mater Sci. 2013;3(4):84-90. doi: 10.5923/j. materials.20130304.04.
High-resolution X-ray microdiffraction analysis of natural teeth.
J Synchrotron Radiat. 2008;15(Pt3):235-8. doi: 10.1107/
36. Fundaoğlu Küçükekenci F, Küçükekenci AS, Çakici F. Evaluation of the preventive efficacy of three dentin tubule occlusion methods against discoloration caused by triple-antibiotic paste. Odontology. 2019;107(2):186-9. doi: 10.1007/s10266-018-0385-y.
37. Kyaw K, Otsuki M, Segarra MS, Hiraishi N, Tagami J. Effect of Calcium-phosphate Desensitizers on Staining Susceptibility of Acid-eroded Enamel. Oper Dent. 2019;44(3):281-8. doi: 10.2341/18-024-L.
38. Gupta T, Nagaraja S, Mathew S, Narayana IH, Madhu KS, Dinesh K. Effect of desensitization using bioactive glass, hydroxyapatite, and diode laser on the shear bond strength of resin composites measured at different time intervals: An In vitro Study. Contemp Clin Dent. 2017;8(2):244-7. doi: 10.4103/ccd.ccd_155_17.
39. Niazy A, Abdul-Hamid ES. Synergistic caries inhibitory effect of a rematerializing agent and CO2 laser on human enamel and root dentin. Cairo Dent J. 2009;25(3):415-24. 40. Friedman S, Liu M, Izawa T, Moynihan M, Dörscher-Kim
J, Kim S. Effects of CO2 laser irradiation on pulpal blood flow. Proc Finn Dent Soc. 1992;88(Suppl 1):167-71. 41. Nair PN, Baltensperger M, Luder HU, Eyrich GK.
Observations on pulpal response to carbon dioxide laser drilling of dentine in healthy human third molars. Lasers
Med Sci. 2005;19(4):240-7. doi:
42. El Assal DW, Saafan AM, Moustafa DH, Al-Sayed MA. The effect of combining laser and nanohydroxy-apatite on the surface properties of enamel with initial defects. J Clin Exp Dent. 2018 May; 10(5):e425. doi:10.4317/jced.54371 43. Lin CP, Lee BS, Kok SH, Lan WH, Tseng YC, Lin FH.
Treatment of tooth fracture by medium energy CO2 laser and DP-bioactive glass paste: thermal behavior and phase transformation of human tooth enamel and dentin after irradiation by CO2 laser. J Mater Sci Mater Med. 2000;11(6):373-81. doi: 10.1023/a:1008986008510. 44. Ahrari F, Mohammadipour HS, Hajimomenian L,
Fallah-Rastegar A. The effect of diode laser irradiation associated with photoabsorbing agents containing remineralizing materials on microhardness, morphology and chemical structure of early enamel caries. J Clin Exp Dent. 2018;10(10):e955-e962. doi: 10.4317/jced.55059.
45. Wang Y, Li X, Chang J, Wu C, Deng Y. Effect of tricalcium silicate (Ca(3)SiO(5)) bioactive material on reducing enamel demineralization: An in vitro pH-cycling study. J Dent. 2012;40(12):1119-26. doi: 10.1016/j.jdent.2012.09.006.
46. Nakagaki S, Iijima M, Endo K, Saito T, Mizoguchi I. Effects of CO2 laser irradiation combined with fluoride application on the demineralization, mechanical properties, structure, and composition of enamel. Dent mater J. 2015;34(3):287-93. doi: 10.4012/dmj.2014-225.
47. Peric TO, Markovic DL, Radojevic VJ, Heinemann RM, Petrovic BB, Lamovec JS. Influence of pastes containing casein phosphopeptide-amorphous calcium phosphate on surface of demineralized enamel. J Appl Biomater Funct
Mater. 2014;12(3):234-9. doi: 10.5301/jabfm.5000194.
48. Mehta R, Nandlal B, Prashanth S. Comparative evaluation of remineralization potential of casein amorphous calcium phosphate and casein phosphopeptide-amorphous calcium phosphate fluoride on artificial enamel white spot lesion: An in vitro light fluorescence study.
Indian J Dent Res. 2013;24(6):681-9. doi:
49. Belcheva A, El Feghali R, Nihtianova T, Parker S. Effect of the carbon dioxide 10,600-nm laser and topical fluoride gel application on enamel microstructure and microhardness after acid challenge: an in vitro study. Lasers Med Sci. 2018;33(5):1009-17. doi: 10.1007/s10103-018-2446-4. 50. Amaechi BT, Higham SM. In vitro remineralisation of
eroded enamel lesions by saliva. J Dent. 2001;29(5):371-6. doi: 10.1016/s0300-5712(01)00026-4.
51. Fekrazad R, Najafi A, Mahfar R, Namdari M, Azarsina M. Comparison of enamel remineralization potential after application of titanium tetra fluoride and carbon dioxide laser. Laser Ther. 2017;26(2):113-9. doi: 10.5978/islsm.17-OR-9.
52. Farhadian N, Rezaei-Soufi L, Jamalian SF, Farhadian M, Tamasoki S, Malekshoar M, et al. Effect of CPP-ACP paste with and without CO2 laser irradiation on demineralized enamel microhardness and bracket shear bond strength.
Dental Press J Orthod. 2017;22(4):53-60. doi:
53. Khamverdi Z, Kordestani M, Panahandeh N, Naderi F, Kasraei S. Influence of CO2 laser irradiation and CPPACP paste application on demineralized enamel microhardness.
J Lasers Med Sci. 2018;9(2):144-8. doi: 10.15171/
54. Reynolds EC, Cai F, Cochrane NJ, Shen P, Walker GD, Morgan MV, et al. Fluoride and casein phosphopeptide-amorphous calcium phosphate. J Dent Res. 2008;87(4):344-8. doi: 10.1177/154405910808700420.
55. Velİ I, Akin M, Baka ZM, Uysal T. Effects of different pre-treatment methods on the shear bond strength of orthodontic brackets to demineralized enamel. Acta Odontol Scand. 2016;74(1):7-13. doi: 10.3109/00016357.2014.982703.